1 Figure 1: Denver International Airport. ABSTRACT As a result of a moderate hailstorm in June of 2001, the original eight-year-old reinforced PVC single-ply membrane on the flat roofs over the Jeppesen Terminal and passenger bridge at the Denver International Airport (DIA) experienced moderate to extensive hail damage. The subject roofs are adjacent to the impressive and renowned Bird Air tent roofs, which were not damaged by the hail. After careful consideration of many different roof systems, the roof membrane was replaced with a non-reinforced, fully-adhered, 90-mil ethylene propylene diene monomer (EPDM) that was painted with a white elastomeric roof coating. The evaluation, design, and construction of the new roof presented the owner, design team, and contractor with some unique challenges and experiences that are shared in this case study. The topics that will be discussed are: 1. Logistics of reroofing an aviation facility and the security challenges of post 9/11/2001, 2. Emergency measures that were taken to prevent further damage to the roof and building components prior to and during construction, 3. Results of the evaluation of the roof systems and existing conditions, 4. The selection process for the new roof membrane, recover board, and roof coating; and 5. Design parameters of the project. For this project, the fully-adhered, 90-mil EPDM roof was determined to be the least intrusive and the best system to provide adequate resistance to hail and mechanical damage. The designers and owners expect the new EPDM roof to provide excellent service in a hail hazard zone and achieve a useful life that far exceeds the norm. Client: City and County of Denver Architect: DMJM H+N, Denver, CO Roof consultant: CyberCon Engineering, Inc., Centennial, CO Roofing contractor: Earl F. Douglass Roofing, Commerce City, CO Product supplier, roofing membrane: Firestone Building Products Corp. Product supplier, coverboard: Georgia Pacific Product supplier, premanufactured coping: Peterson Aluminum 16 INTERFACE S EPTEMBER 2005
2 INTRODUCTION This article will discuss the results of CyberCon s initial investigation of the roofs at the DIA, design considerations for reroofing, and some of the challenges that were encountered during the reroofing process. This paper will also discuss the characteristics, physical properties, and some of the pitfalls of the roofing products used and the rationale for selecting an elastomeric thermoset roofing membrane and dense, water resistant coverboard for reroofing. For most discerning readers, the information provided will be a quick refresher on polymer chemistry, mechanics of materials, moisture vapor transmission, thermal properties, and sound roofing practice. For the roof consultant in training, it is hoped that the information provided will inspire further study of the topics discussed. DIA is a commercial air carrier facility 23 miles northeast of the metropolitan Denver area, on 34,000 acres of the high mountain desert prairie of Colorado. The airport has six active runways and handles approximately 104,000 enplanements each day. The terminal and concourse facilities represent a total of 5.45 million square feet with a total of 94 passenger-loading gates. The airport structures consist of a main terminal and three remote concourse buildings (A, B, and C), which are connected via an underground automated transportation system. Concourse A is connected to the North terminal via a pedestrian bridge. An international airport presents challenges that are unique due to its 24/7 operations, ongoing public activity, security, and the sensitive nature of the airplanes. Special considerations are necessary for reroofing to address noise, odors, and risks to the operations of the facility. Our findings and conclusions from the investigation of the original roof systems may also be of interest to the reader. The following will be discussed in more detail in the body of this article: Hail damage to weathered reinforcement PVC membranes. PVC degradation as a function of its environment and raw materials. Designing resistance to mechanical damage of a membrane. Long-term serviceability of a PVC membrane. Slip sheet damage below mechanically fastened single-ply membranes. Premature plasticizer migration. Heat degradation of polystyrene. S EPTEMBER 2005 Vapor diffusion and degradation of polyisocyanurate. Thermal profile of black EPDM membrane versus a high albedo coating. Failure of butyl-based glued seams on an elastomeric membrane. In the final analysis, it was determined that a fully-adhered EPDM membrane, coated white, installed over a glass-faced gypsum coverboard, mechanically fastened over the existing polystyrene and polyisocyanurate rigid insulation, would be the best reroof option for the DIA. The new roof has passed severe hail and wind tests and has excellent weathering characteristics. It is anticipated that the roof coating will weather away at approximately 1 mil per year and therefore have to be reapplied in approximately 12 to 15 years. The serviceable life of the roof should extend well beyond 30 years. The life cycle cost was deemed to be comparable to other membrane systems, despite the anticipated cost of recoating the roof. The rationale for selecting an EPDM roof system will also be discussed in this article. DEFINITIONS Absolute Humidity A measure of the actual amount of water vapor contained in a unit volume of air; distinct from relative humidity, which is the ratio of air s absolute humidity to the air s water vapor holding capacity. 9 Diffusion The process whereby water vapor or gases migrate through permeable membranes or partitions by osmosis. Gases always migrate from regions of high concentrations to regions of low concentrations until equilibrium is reached. Elastomer A macromolecular material that, at room temperature, returns rapidly to approximately its initial dimensions and shape after substantial deformation by a weak stress and release of the stress. 4 Glass Transition Temperature The temperature at which a polymer becomes brittle, and above a certain point, the polymer is deemed prone to failure. 2 Plasticizer An important component in the formulation of PVC membranes to give them flexibility to withstand elongation, strain, and thermally-induced stresses normally experienced by a roof system. Most plasticizers are esters of phthalic acid. The molecular weight and compounds vary from one manufacturer to the next. The plasticizer content in a new membrane is around I NTERFACE 17
3 PROBLEMS WITH THE EXISTING ROOF SYSTEMS SYSTEM NO. EXISTING CONDITIONS: OBSERVATIONS: 1. Low-slope Deck: Structural concrete (sloped at 1/4"/ft.) Extensive hail damage and mechanical damage areas of Insulation: 4" of extruded polystyrene (XEPS) from icicles falling off of tent roof terminal, east Slip Sheet: Manninglass felt Plasticizer loss and west of Membrane: 60-mil reinforced mechanically-attached PVC Damaged slip sheet the tent roof Thermal degradation of PVC Isolated heat degradation of polystyrene Minor corrosion of fasteners Consolidation of insulation in high-traffic areas 2. Low-slope Deck: Structural concrete (flat) Extensive hail damage roofs on North Insulation: Tapered XEPS 4.5" start, (sloped at approximately Plasticizer loss Terminal and 1/4"/ft.), total maximum thickness 16" Damaged slip sheet Customs areas Slip Sheet: Manninglass felt Membrane: 60-mil reinforced mechanically-attached PVC Thermal degradation of PVC Isolated heat degradation of polystyrene 3. Mechanical Deck: Metal (sloped at 1/4"/ft.) Minor hail damage and elevator Barrier Board: 5/8" Type X gypsum Plasticizer loss penthouses at Insulation: 2 layers of XEPS, 1" and 3" for a total thickness of 4" Damaged slip sheet terminal Slip Sheet: Manninglass felt Membrane: 60-mil mechanically-attached PVC Thermal degradation of PVC 4. Steep-slope Deck: Structural concrete (sloped at 3"/ft.) Extensive hail damage areas of Insulation: 2.6" polyisocyanurate Plasticizer loss Terminal East Membrane: 60-mil mechanically-attached PVC Thermal degradation of PVC and West Minor corrosion of fasteners Minor facer delamination 5. Passenger Deck: Metal (sloped 0" to 3"/ft.) with fireproofing on bottom Extensive hail damage bridge (slope side Plasticizer loss 0" to 1"/ft.) Barrier Board: 5/8" Type X gypsum Thermal degradation of PVC and barrel roof Insulation: 2.6" of polyisocyanurate over Customs Slip Sheet: Manninglass (0" to 3"/ft.) Membrane: 60-mil mechanically-attached PVC 6. Airport Deck: Structural Concrete (sloped at 1/4"/ft.) Severe buckles and deformation of Operations Insulation: 2.6" polysiocyanurate mechanically attached polyisocyanurate Building (AOB) Membrane: Fully-adhered.060" un-reinforced EPDM Severe facer delamination above 10th Degradation of insulation cell structure (1/4" to floor offices 1/2" of the top layer turned brown and friable). Extensive failure of adhesive seams Corrosion of fasteners 7. AOB Penthouse Deck: Metal (sloped at 1/4"/ft.) fireproofing on bottom side Insulation: 2.6" polysiocyanurate, mechanically attached Membrane: Fully-adhered.060" unreinforced EPDM Deterioration of lap sealant The rigid insulation was deemed salvageable 8. AOB 6th floor Deck: Structural concrete (flat) Buckles and deformation of polyisocyanurate offices Insulation: Tapered polyisocyanurate (4" start, sloped at approximately 1/4"/ft.) Membrane: Fully-adhered.060" unreinforced EPDM Isolated facer delamination Degradation of insulation cell structure (1/4" to 1/2" of the top layer turned brown and friable). Failure of adhesive seams Minor corrosion of fasteners Table 1: Problems with existing roof systems. 36%. A loss of 10 to 12 percent can result in premature failure of the roof system. Low molecular weight plasticizers are more volatile than those that have higher molecular weight INTERFACE Thermoplastic A material that becomes plastic or viscous when heated and semi-rigid when cooled. Asphalt and PVC are classic thermoplastic materials. BACKGROUND Construction of DIA The construction of the terminal and Airport Operations Building (AOB) was completed in 1991 and the passenger S EPTEMBER 2005
4 Figure 2: Hail-damaged membrane. bridge was completed in The roofs on the terminal, AOB, and passenger bridge were replaced in Eight different roof systems were identified. The following is a brief description of the roof system components and the type of problems noted. DISCUSSION Thermoplastic PVC Membranes As early as 1999, only eight years after the original roof was installed, the PVC roofs on DIA began showing signs of degradation and premature plasticizer loss. Melting of the extruded polystyrene rigid insulation was also noted, particularly in super insulated areas with southern exposure to the sun. In June of 2001, a moderate hailstorm hit the airport, causing extensive damage to the PVC membrane on the terminal. The membrane did not shatter (unlike some of the first-generation PVC roof systems); however, concentric cracks were noted in the membrane at points of hail impacts. In most cases, the cracks ran completely through the membrane, rendering the roof system unsuitable as a waterproofing system. In some instances, the cracks emanated from the underside of the single-ply membrane, but did not manifest on the top or exposed side of the membrane. The damage noted was more extensive on the darker discolored sheets used to construct the PVC membrane, (which apparently had different run numbers), and in areas that were exposed to more solar radiation. New cracks developed in the membrane at hail impacts that were not noticeable during the first visual inspection. The visible cracks were repaired immediately with EPDM primer and EPDM peel-andstick flashing tape. The repairs were paint 20 INTERFACE ed white to prevent thermal degradation of the polystyrene insulation below. Frequent inspections were performed to identify new cracks and to effect repairs to prevent water infiltration through the existing single-ply membrane. Fortunately, the re-roof project was performed during a drought, which was recorded as the driest period in the previous 50 years. The original roof system specified and installed on the vast majority of the buildings at DIA was an off-white, 60-mil, polyester scrim reinforced, mechanically-fastened PVC single-ply membrane, which was produced using the calendaring process. PVC is a thermoplastic material, which means that it becomes softer (or more plastic) with heat and semi rigid with cold. PVC is known for its resistance to acids, alkalis, and many other chemicals, as well as its self-extinguishing properties when subjected to fire. It is soluble in certain solvents, such as tetrahydrofuran, which is used in PVC cements. 3 One of the main reasons PVC was used on the airport is that it was perceived that the membrane might be exposed to jet fuel. It was also one of the few membranes on the market that had a UL fire rating for all roof slopes encountered at the airport. The membrane, with its heat-welded and solvent seams, was also touted to be superior to other conventional roof systems, despite the lack of a longterm performance history. Much has been learned about thermoplastic PVC single-ply membranes since they were introduced in the U.S. from Europe in the late 1970s. The non-reinforced sheet is no longer produced or marketed due to the shattering phenomenon and hail damage that occurred with the product. All of the sheet goods marketed and sold in the U.S. today (except for flashing materials) are reinforced with polyester or fiberglass mats or scrims, which have greatly improved the dimensional stability of the original non-reinforced products. The membrane can be manufactured white or tinted in various colors with pigments, which is an advantage when solar reflectivity or an architectural statement is desired. The heat welding of the seams, using hot air welders, is also fairly consistent and reliable. PVC copolymers in their normal state are rigid, brittle, and easily shatter under stress. Plasticizers, fillers, pigments, processing oils, biocides, and stabilizers are compounded with the PVC resins to impart the desired physical properties to the membrane. Plasticizers are used to give the sheet flexibility and suppleness over a wide range of temperatures. Stabilizer packages are introduced to provide resistance to thermal and photochemical degradation. Plasticizers begin to migrate out of the sheet and the chemical bonds begin to change as soon as the membrane leaves the production line. This phenomenon, known as weathering, is normally a very slow and gradual process, which under favorable conditions, allows a PVC membrane to provide a useful life commensurate with other conventional roof systems. The glass transition temperature and specific gravity are increased and shrinkage of the membrane occurs as a result of thermal degradation and plasticizer loss. Exposure to heat, ultraviolet radiation, and various absorbent Figure 3: Patches from hail damage. compounds will accelerate the degradation of PVC. Thermal degradation is manifested by a brown color, as the membrane goes through dehydrochloronation of the polymer. 2 Plasticizer loss occurs by migration, evaporation, washout, hydrolosis, and exposure to microbes. 1 S EPTEMBER 2005
5 Polystyrene rigid insulation (which was used extensively on the airport) has an affinity for PVC plasticizers; therefore, the two roof components must be adequately divorced for the duration of the roof s useful life. PVC membranes should also be adequately divorced from asphalt-contaminated surfaces for the same reason. As PVC weathers, it loses some of its elasticity and flexibility. It has been demonstrated that new PVC membranes will generally produce a tensile load of 4-6 pounds per inch when subjected to a 100 F temperature drop. As the membrane weathers and becomes more brittle, the thermal load profile can increase fourfold to 20 plus pounds per inch. 1 It has been suggested that the shrinkage and thermal load profile of a PVC membrane can be affected by the manufacturing process and raw materials used in the products. 2 The extent of the effects from manufacturing is beyond the scope of this article. The shattering phenomenon that occurred with the first generation PVC nonreinforced membranes can be attributed to plasticizer loss, shrinkage, lack of flexibility, and increased thermal loads during sudden drops in temperature. Hail and impact damage to reinforced thermoplastic membranes can also be attributed to the same changes in physical properties; however, the mat or scrim prevents a weathered membrane from shattering into thousands of smaller pieces. Isolated cracks through the membrane, generally in the form of concentric circles, are usually noted after a hail event or impact, which compromises the watertight integrity of the membrane. The kinetic energy of a missile is converted to strain energy in the membrane, compressive yield stress in the substrate, disintegration of the missile, and momentum after impact. Hailstorms are usually preceded by a sudden drop in temperature, which, as discussed above, causes the membrane to shrink, resulting in thermally induced loads in the material. At the moment of impact, the membrane begins to deform, and, as with any material under load, develops additional tensile stresses on the underside and compressive stresses on the top side of the membrane. If the strain exceeds the elastic limit of the material at the time of impact, cracks begin to emanate from the bottom side toward the top surface. An underside view of the membrane is needed to ascertain the full extent of hail damage, since cracks may develop but not penetrate completely through the membrane. Impact resistance of the membrane can be improved by providing a denser substrate below the membrane, which resists deformation and elongation, thus minimizing the strain energy imparted to the membrane. Bridged or unsupported areas are still vulnerable to damage. The long-term serviceability of a PVC roof membrane is a function of its dimensional stability and flexibility throughout the temperature range it will experience during its anticipated serviceable life. The stability of these physical properties is a function of the raw materials, manufacturing process, and environment to which the roof system is exposed. Polystyrene Rigid Insulation The vast majority of insulation used on the original roof at the airport was extruded polystyrene, which ranged in thickness from 4" (R-20 on structurally sloped areas) to 14" (R-20 to R-70 on the flat decks with tapered insulation). Most of the insulation board was deemed salvageable, which represented a sizeable investment by the owner, the city, and the county of Denver. S EPTEMBER 2005 I NTERFACE 21
6 Figure 4: Melted XEPS. The new roof system had to be compatible with the existing polystyrene rigid insulation. A new, ballasted, single-ply membrane over a coverboard would have been an economical choice on any other project. The owner s choice to eliminate any roof system with loose rocks, which could become missiles during high winds, was respected and other reroof options were considered. Extruded polystyrene is a plastic foam, closed-cell rigid insulation with a fluorocarbon blowing agent. The polymer that makes up the cell walls is relatively impermeable to water vapor, which renders the product useful in areas that may become exposed to moisture, (i.e., foundation walls, roofs, wall cavities, protected membrane roof assemblies, etc). It has a fairly stable aged R-value of 5.0 per inch. Extruded polystyrene is considered a sustainable roofing product and can be salvaged for subsequent membrane replacements, under favorable conditions. The product has a published service temperature range of -100 to 165 F; therefore, it must be protected from temperatures above this range. This can be accomplished with slip sheets, coverboards, and reflective membranes or coatings. Polystyrene will disintegrate when exposed to various solvents, including membrane adhesives, cold process cements, and other petroleumbased chemicals. A limited number of adhesives are suitable for laminating polystyrene boards to one another and to other products. Solvent-free, rubberized emulsion adhesives have been developed that are compatible with polystyrene. When the existing membrane was removed, it was noted that some of the 22 INTERFACE extruded polystyrene rigid insulation boards had melted or deformed from heat, particularly where the slip sheet was damaged or missing, and in areas next to the reflective clerestory windows (refer to Figure 1 for view of window areas). To melt extruded polystyrene, the temperature needs to reach 165 F or greater, according to the manufacturer s published literature. The ambient air temperature directly above the membrane was noted to be 95 F on a hot summer day. The melting indicates that the temperature between the membrane and the polystyrene exceeded the air temperature by 60 F to 70 F, which is incongruous with static thermo profiles of building envelopes that have been presented in the past. The slip sheet protected the polystyrene somewhat, but did not prevent deformation of the insulation board. Insulation boards that were severely deformed or melted were replaced with like kind. A single layer of 5/8" glass-faced gypsum board with a primed surface was installed over the existing polystyrene rigid insulation (secured with mechanical fasteners and Galvalume metal plates) to provide a dense, hail-resistant substrate for the new membrane and divorce the polystyrene from the elevated temperatures that were anticipated with the new black EPDM membrane. A couple of isolated areas, near clerestory reflective windows, experienced some heat degradation and had to be repaired (Figure 4). The new black EPDM membrane was painted white to lower the surface temperature of the roof during the hot summer months, which will prevent the polystyrene from melting. During reroofing (after the new black 90-mil EPDM membrane was installed, and prior to the application of the white elastomeric coating), and when the ambient air temperature reached or exceeded 100 F, some severe deformation in the underlying polystyrene rigid insulation occurred in isolated areas (next to intersecting clerestory windows). The surface temperature of the black EPDM membrane was measured at 180 F at approximately 1:30 p.m. on a hot summer day. The membrane in these areas, next to the reflective windows, received much more solar radiation than other areas of the roof. As soon as the high-albedo, white roof coating was installed, the surface temperature dropped significantly to approximately 105 F, which prevented any further damage to the top layer of the polystyrene rigid insulation board. Polyisocyanurate Rigid Insulation Polyisocyanurate rigid insulation (PRI) with a permeable organic facer was used on some areas of the airport. When the roof was installed, hydrochlorofluorocarbons (HCFCs) were used as blowing agents for the plastic foam insulation boards. Various roof systems, using this product, were encountered: Mechanically-fastened reinforced PVC membrane over a single uniform layer of PRI over a structurally sloped concrete deck. Mechanically-fastened reinforced PVC membrane over a single uniform layer of PRI over a structurally sloped metal deck. Fully-adhered non-reinforced EPDM membrane over tapered PRI boards, mechanically fastened over a flat concrete deck. Figure 5: Damaged oxidized polyisocyanurate. S EPTEMBER 2005
7 Fully-adhered, non-reinforced EPDM membrane over a single uniform layer of PRI, mechanically fastened over a structurally-sloped concrete deck. Fully-adhered non-reinforced EPDM membrane over a single uniform layer of PRI, mechanically fastened over a metal deck. On the concrete deck areas, several problems (moderate to severe) were noted that were not evident on the metal deck areas. The organic facer was deteriorated, the membrane was delaminated from the facer, the insulation board was buckled in a convex fashion, the top 1/4" layer of the board was discolored and friable, the insulation fasteners and plates were corroded, and the glued EPDM seams were delaminated (refer to Figure 5). Each one of these problems can be attributed to the effects of moisture. Residual water from the pouredin-place concrete was the probable source of the initial moisture, causing the EPDM seams to fail within a relatively short time, which precipitated the damage to the insulation board and fasteners. More water entered the roof system via open seams, which exacerbated the deleterious effects of moisture on the roofing components. There was evidence that patches and repairs were made when leaks occurred, but the residual moisture was probably not removed. The facer is a critical and integral part of polyisocyanurate rigid insulation products. It provides dimensional stability and fire resistance to the insulation board and a means to adhere a roof membrane to an otherwise unstable and friable material. If organic facers become wet, the fibers expand, allowing the dimensionally unstable plastic foam board to expand or contract, resulting in bowing or cupping of the board. When the cellulosic facer dries, it shrinks, imparting stress on the board. If the roof system goes through enough wetting and drying cycles, the structural integrity of the facer becomes compromised and a fully-adhered membrane will eventually become disbonded. Polyisocyanurate foam is a cellular plastic insulation that entraps a gaseous blowing agent within microscopic cells of a polymer matrix. The cells of the foam are primarily closed, and due to the low thermal conductivity of the entrapped gas, the foam is an effective insulator. The cell walls are permeable and, with time, the blowing agent(s) can escape from the cells while ambient gases such as N 2, O 2, and H 2 O vapor diffuse relatively quickly through the cell walls and permeate the foam. The resulting change in the gas composition of the foam over time, and the corresponding decrease in its insulating capability, are referred to as aging of the foam. 8 Studies have shown that in the presence of heat and moisture, the aging process of plastic foam insulation products is accelerated and the physical properties thermal conductivity, compressive strength, density, coefficient of linear expansion, and vapor permeability are affected substantially above 120 F (49 C). Under dry conditions, polyisocyanurate foam insulation is dimensionally stable (<5% change in dimension and <15% by volume) up to 220 F (104 C). At temperatures above 120 F (49 C) and a relative humidity above 90%, the Figure 6: Psychrometric chart, courtesy of RIEI. product becomes dimensionally unstable: (5 to 20% dimensional changes in each direction and 15 to 60 percent change in volume can occur). 1 Over wet substrates, weathering, moisture gain, and dimensional changes in polyisocyanurate foam insulation products tend to be more pronounced with dark roofs, due to the elevated temperatures. The designer or installer of a roof system should properly evaluate the presence of moisture. Nondestructive moisture evaluations are highly recommended for recovers where trapped moisture is probable. Cementitious decks should be checked for moisture content if a vapor retarder is not used or specified. On new construction, vapor retarders are recommended over concrete decks to prevent the residual moisture from affecting the roof system components. Studies are being done on the drying effects of loose-laid, pressureequalized venting single-ply roof systems. The long-term viability is still being researched. 11 Water vapor always diffuses from regions of high absolute humidity to regions of low absolute humidity. The greater the difference in absolute humidity across a permeable structure, the faster the rate of 24 INTERFACE S EPTEMBER 2005
8 YEAR OF INTRO: TECHNOLOGY IMPROVEMENTS Butyl-based splice adhesive replaces water- and heatsensitive Neoprene-based adhesives EPDM-based wall flashings replace heat- and ozone-sensitive Neoprene-based flashings Tape laminates replace adhesive seams at roof edges and battens Metal battens and screw fasteners replace treated wood nailers and nails at base tie-ins Reinforced perimeter fastening strips introduced as an alternative to metal battens for base tie-ins Seam tape with high solids primer replaces seam adhesive. Table 2 diffusion. Thickness of a material also affects the permeability or rate of diffusion. In most building situations, warm air tends to have a higher absolute humidity than cooler air. This gives rise to the adage, water vapor goes from hot to cold. This is not necessarily true for buildings with unusually high or low interior humidity or buildings with wet or moisture-laden components. Water vapor migration is usually not a concern until the gaseous molecules reach the dewpoint temperature and condense into liquid water. 10 Foam insulation products can become wet by vapor diffusion followed by condensation. Water accumulates in the foam when vapor drive acts in concert with thermal gradients and the vapor is restricted on the cold side of the building envelope. Moisture accumulation is reversible, which means foam insulation can eventually dry out, if allowed to, by vapor diffusion. On the airport project, evidence shows that the permeability of the EPDM membrane was not sufficient to allow adequate amounts of water vapor to escape to the atmosphere. The polyisocyanurate rigid insulation and facer at the DIA project experienced numerous cycles of wetting and drying as a result of the residual moisture trapped between the deck and black EPDM membrane. The black membrane reached temperatures of 180 F in the summer, which increased the thermal gradient, vapor pressure, and therefore, the vapor diffusion rate, thereby accelerating the degradation of the foam insulation and facer on the top side of the boards. This, however, S EPTEMBER 2005 would not explain the brown discoloration of the top surface of the insulation board (refer to Figure 5), which is usually indicative of photochemical oxidation. The solvents in the bonding adhesive, in concert with moisture and heat, may have reacted with the polymer matrix of the insulation board. Further study is needed. This demonstrates the need for a vapor retarder over freshly-poured (moisture-laden) concrete decks. Elastomeric EPDM Single-ply Membranes EPDM is an elastomeric thermoset polymer synthesized from ethylene propylene and a small proportion of a diene monomer with rubber-like or elastic properties. The black membrane, which has carbon black as a UV inhibitor, has excellent weathering characteristics. EPDM is not resistant to petroleum oils and gasoline. 3 The membrane will swell and soften when exposed to these chemicals. Other than silicone, EPDM has the best service temperature range of any elastomeric membrane on the market (-65 to 300 F). A non-reinforced membrane has a tensile strength of 1400 lbf/in 2 and an ultimate elongation of 300%. EPDM also performs very well under heat and exposure to ozone. EPDM membranes have a proven track record. Due to improved product technology and superior details, problems with shrinkage and failed seams have greatly diminished since the product was first introduced to the roofing market more than 25 years ago. 12 It was decided that a black, 90-mil, nonreinforced EPDM membrane would be I NTERFACE 25
9 ROOF REPLACEMENT OPTIONS Built-up roof SBS modified, hotor cold-applied PROS AND CONS Rejected because of asphalt fumes, loose rock, and potential for melting existing polystyrene. Rejected because of asphalt or solvent fumes and potential for melting existing polystyrene. High Albedo White Roof Coating A white roof coating was specified and installed to lower the surface temperature of the roof in order to prevent the polystyrene rigid insulation from heat degradation. The coating also provides the following benefits: Encapsulates all seams and edges of the membrane and flashing materials, thereby providing additional redundancy in the waterproofing system. Protects the membrane and flashings from heat and UV exposure, extending service life. Greatly reduces the temperature gradient of the roof, which lowers the relative humidity and vapor drive within the roof system components. Provides an aesthetic appearance to the roof. APP modified, torch or cold-applied PVC TPO EPDM ballasted EPDM mechanically attached EPDM fully-adhered installed over a layer of 5/8" glass-faced gypsum board, which was mechanically fastened over the existing salvaged polystyrene rigid insulation. The only drawback perceived with the EPDM roof on the airport was its black color, which gets hot during the summer months from solar radiation. The temperatures would get hot enough to cause deformation of the existing polystyrene insulation board. White EPDM, which has a titanium dioxide UV inhibitor, was rejected because the product does not have the same weathering properties as black EPDM, which uses carbon black. It was decided to coat the roof with approximately 15 mils of a high albedo white acrylic elastomeric roof coating, after washing and priming the membrane. Prior to coating, seams of the EPDM sheets were mated with 3"-wide butyl seam tape and a high-solids, butyl-based primer. The seams were then covered with a 5"-wide, butylbacked, self-curing EPDM flashing tape. This seaming method provided redundancy and ensured that any small pinholes particularly at tee joints were sealed watertight for the serviceable life of the roof membrane. The hail and puncture resistance are excellent with EPDM when installed over a 26 INTERFACE Rejected because of risk of open flames and the negative effect of solvent fumes on polystyrene. Rejected because of past experience at airport. Rejected because of limited performance history. Rejected because of loose rock or pavers. Rejected because of dynamic forces on membrane and fasteners and noise from the extensive use of fasteners. Accepted because of durability, low life cycle cost, excellent resistance to wind and hail, and minimal intrusion on facility operations. Table 3 hard board. The fully-adhered EPDM over 5/8" glass-faced gypsum board has passed the most severe hail tests and has received the highest ratings from United Laboratories (UL), the National Institute of Standards and Technology (NIST), and Factory Mutual (FM) for hail resistance. A 2" hail warranty was issued by the roofing manufacturer. The membrane installation was rather innocuous, but some precautions were needed to avoid adhesive fumes from being drawn into the building through the fresh air intakes of the mechanical air handling system. Plywood chutes eight feet high were built around the fresh air intakes and were very effective. It is anticipated that the coating will weather at the rate of 1 mil per year. This gradual chalking process is what keeps the roof white and highly reflective for the life of the coating. It is anticipated that the roof may need to be recoated at least once during its useful life. The cost of the coating is offset by the savings achieved from the extension of the useful life and reduced energy consumption during the summer to condition the air in the building. The peel strength and adhesion of water-based acrylic roof coatings have improved greatly since primers or prewashes were introduced. Practically all manufacturers of roof coatings and EPDM membranes offer white coating specification and warranties. The prewash was lightly sprayed on the surface of the finished EPDM roof and then rinsed off with water. After the membrane dried, the water-based coating was applied with rollers. To avoid overspray, a spray apparatus was not used. Water-based acrylic coatings perform best on roofs with adequate slope and drainage. Ponding water will cause the coating to swell and peel away from the membrane. When exposed to standing water for prolonged periods, moisture will be absorbed into the coating, causing dimensional changes. This induces shear stress at the adhesive bond. If the water absorbed into the coating freezes, the coating will break down and eventually delaminate from the substrate. ROOF SYSTEM SELECTION PROCESS Owner s Concerns As one can imagine, the facility management and engineering staff had several concerns and expectations with regard to the new roof systems. With the exception of one roof area (System No. 7), the original roofs did not perform as anticipated and had to be replaced prematurely due to hail damage and degradation of the physical properties of the polyisocyanurate rigid insulation and PVC roof membranes. The manufacturer s roof guarantee did not cover hail damage, and the manufacturer would not participate S EPTEMBER 2005
10 in replacing the roof because of the change in the membrane s physical properties and likelihood of further hail damage. Because of the premature degradation of the PVC membrane, foot traffic on the roofs had to be limited to times when the outdoor ambient temperature was 40 F or above. The design team had to come up with a roof that would address the following issues: Heat Aging: The high R-values (super insulated roof at apex of tapered insulation system) and the reflective glass on the clerestory windows places the membrane in an environment with abnormally high heat and solar radiation. The new membrane must have good heat aging properties. Sustainable: The new roof system must be compatible with the existing polystyrene insulation boards. A large investment had already been made with the thermal insulation and tapered system. Low Meltpoint of XEPS: The temperature of the membrane must remain well below the melt point of the polystyrene insulation board. Hail Resistance: The new membrane must be proven to withstand hail. Facility Operations: The roof replacement process must be as non-intrusive as possible, and the finished roof must not utilize looselaid components that could become missiles in the event of a tornado or high winds. Removing the polystyrene rigid insulation also posed a high risk for the tarmac operations, particularly on windy days. Maintenance: The roof system should be easy to repair and require little maintenance. Temperature Limitations: The adhesives and products must be workable during all four seasons of the year, due to the long duration of the project. Options Presented to Owner Several roof replacement options were presented to the airport staff. The pros and cons were discussed for each roof type. 28 INTERFACE PROJECT CHALLENGES The first and foremost challenge was selecting a roof system that would be as unintrusive and risk free as possible for the facility operations and customers of the airport. The transfer of materials on and off of the roof had to be minimized and the roofing products had to be rather innocuous. By salvaging the majority of the existing insulation board, the owner enjoyed cost savings as well as reducing the risk of debris blowing onto the tarmac. Security issues were paramount, especially after the September 11, 2001, terrorist attack on the U.S. The contractor had to provide a sufficient number of laborers who could pass the stringent screening methods imposed by the government. Even moving tools onto the jobsite was cumbersome. Personnel on the roof had to be badged and escorted by qualified persons. Staging was limited and difficult. The airport officials required that staging plans be submitted and approved weeks in advance. Most of the material and debris handling was done at night. Underground tunnels and buildings precluded crane setups to specific areas. Special cranes with long booms were utilized to move materials on and off of the ten-story Airport Operations Building. Debris, flammable goods, and loose materials could not be stockpiled on the roof. Products and materials that were not properly bundled together had to be removed from the jobsite at the end of each day. Some parapet wall sections were curved. New sections of coping had to be Figure 7: Return air chutes. custom fabricated and pre-finished. Each curved section had to be measured with a template and shipped to the metal supplier for fabrication. Over 100 different coping sections had to be custom made. The roof had to be installed during dry and warm weather because of the waterbased roof coating, which is subject to damage from freezing prior to curing. The established schedule was from April to Novem- ber. Over 4,000,000 square feet of roofing had to be installed in six months. Return air intakes were located near the roof level, which presented a potential problem with offensive solvent fumes being drawn into the air handling units and dispersing them into the occupied building. Plywood chutes were constructed around the intakes and anchored with tie-backs to resist wind pressures. This precaution was deemed effective, and no complaints were received with regard to the solvent fumes (refer to Figure 7). CONCLUSIONS Weathered reinforced PVCs are subject to hail damage. In hail zone areas, designers should consider a hard coverboard that offers more resistance to impact deformation and lowers the strain energy imparted to the membrane. Polystyrene rigid insulation is subject to heat degradation, even when a light-colored membrane and slip sheet are provided, particularly when exposed to extraordinary solar radiation that occurs with reflective clerestory windows. Fiberglass slip sheets are subject to damage on mechanically-fastened, singleply roof systems due to fluttering of the membrane on windy days. Slip sheet displacement will result in premature plasticizer migration of PVC over polystyrene. High thermal R-values and solar reflection from windows accelerate weathering of a PVC roof membrane, resulting in premature plasticizer loss and degradation. S EPTEMBER 2005
11 Manufacturing processes, compounds, and environmental exposure can have a major affect on long-term flexibility and serviceability of PVCs. Generally, polyisocyanurate rigid insulation products perform very well under extreme heat or temperatures often experienced in a roof assembly, even when installed below dark or black membranes which can achieve surface temperatures of 180 o F. When moisture is introduced and becomes trapped in the insulation from membrane leaks, vapor diffusion, or residual water in cementitious roof decks, the weathering and degradation of polyisocyanurate rigid insulation are intensified. In such instances, the physical properties and dimensional stability of polyisocyanurate rigid insulation are eventually compromised, and the sustainability of the product is negated. Concrete decks on new construction are apt to contain large amounts of residual moisture that can have a deleterious effect on some plastic foam insulation products, organic facers, and adhesive seams of elastomeric membranes. Designers and installers should consider vapor retarders over moisture-laden concrete decks to prevent moisture migration and condensation within an insulated roof assembly. Construction traffic can cause scarring of the roof membrane that will cause latent problems post construction. The product quality and long-term serviceability of roof membranes differ greatly among manufacturers. In the selection process of a roof system, there is no substitute for time-proven performance. To be successful, difficult projects require extraordinary planning, synergies from all parties, cooperation, and constant open lines of communication. REFERENCES and FURTHER READING 1. Dr. H.O. Laaly, The Science and Technology of Traditional and Modern Roof Systems, Volume 1. Los Angeles: Laaly Scientific Publishing, Ralph Paroli, Brian Whelan, and Thomas Smith, Shattering of Unreinforced PVC Roof Membranes: Problem Phenomenon, Causes and Preventions, Proceedings of NRCA/ NIST Tenth Conference on Roofing Technology, April 22-23, 1993, pp , NRCA, Rosemont, IL.
12 3. Walter Rossiter Jr. and Robert Mathey, National Bureau of Standards, Elastomeric Roofing, Roofing/ Siding/Insulation, Harcourt Brace Jovanovich, Inc., September American Society for Testing and Materials, Standard Definitions of Terms Relating to Rubber, ASTM Designation D a, 1977 Annual Book of ASTM Standards, Part 37, Philadelphia, Pennsylvania, American Society for Testing and Materials, ASTM C-755; Standard Recommended Practice for Selection of Vapor Barriers for Thermal Insulations, ASTM C-755, Philadelphia. 6. N.V. Schwartz, M. Bomberg, and M.K. Kumaran, Water Vapor Transmission and Moisture Accumulations in Polyurethane and Polyisocyanurate Foams, Water Vapor Transmission Through Building Materials and Systems; Mechanisms and Measurements, ASTM, Philadelphia, American Society for Testing and Materials, Standard Specification for Poly(Vinyl Chloride) Sheet Roofing, ASTM D-4434, Philadelphia. 8. R.R. Zarr and T. Nguyen, Effects of Humidity and Elevated Temperature on Density and Thermal Conductivity of a Rigid Polyisocyanurate Foam, Proceedings of the SPI 34th Annual Polyurethane Technical/Marketing Conference, October Moisture Vapor Transmission, The Society of the Plastics Industry, Inc., Polyurethane Foam Contractors Division, Washington, DC ASTM E-96, Standard Test Method for Water Vapor Transmission of Materials, ASTM, Philadelphia. 11. Warren R. French, Post Installation Field Evaluation of a Pressure- Equalized Single-ply Roofing System to Determine Drying Effects on a Moist Cementitious Roof Deck, Interface, Roof Consultants Institute, August James L. Hoff, EPDM Roof System Performance: An update of Historical Warranty Service Costs, Interface, Roof Consultants Institute, September Jim D. Koontz and Vickie Crenshaw, Simulated Hail Damage and Impact Resistance Test Proceedures for Roof Coverings and Membranes, Interface, Roof Consultants Institute, May This article, originally entitled, Reroof Project Case Study: Denver International Airport Terminal Flat Roofs, was presented as a part of the 19th RCI International Convention & Trade Show in April 2004 in Reno, Nevada. Nick A. Lovato Nick Lovato is president of CyberCon Engineering Inc., a roofing and waterproofing consulting firm founded in He graduated from the University of New Mexico with a B.S. in civil engineering and has 25 years of professional experience in roofing, including technical sales support, roof consulting, and construction management. Mr. Lovato has been a member of the Roof Consultants Institute since 1992 and is a past director of Region V. Nick resides in Littleton, Colorado with his wife Candace.
BUILDING TECHNOLOGIES PROGRAM Guidelines for Selecting Cool Roofs July 2010 V. 1.2 Prepared by the Fraunhofer Center for Sustainable Energy Systems for the U.S. Department of Energy Building Technologies
Measure Guideline: Basement Insulation Basics R. Aldrich, P. Mantha, and S. Puttagunta Consortium for Advanced Residential Buildings October 2012 NOTICE This report was prepared as an account of work sponsored
Risk Control Bulletin Water Damage Prevention A Property Protection Imperative Water is one of the most destructive agents when released into a building. Water erodes surfaces; causes rot and deterioration
Roofing Solutions Reference Manual for Property Managers, Owners, Architects, and Specifiers US$19.95 Money-saving roof restoration options Why problem prevention is your best value How roof maintenance
Underwater Bridge Repair, Rehabilitation, and Countermeasures Publication No. FHWA-NHI-10-029 Pre-Publication Edition NOTICE This document is disseminated under the sponsorship of the Department of Transportation
CertainTeed Shingle Applicator s Manual Shingle Underlayments and Flintlastic SA 5 Roof Systems YOUR OBJECTIVE: To learn the differences between the various underlayments available. To learn when a particular
knk5 Z?m1Z Government of Nunavut Nunavut Kavamanga Gouvernement du Nunavut Good Building Practices Guideline Second Edition December 2005 FOREWORD Building in the North is indeed different than building
Avoidance of Mold Avoidance of Mold Introduction Architects and engineers need to consider the potential for mold growth in all phases of building design, construction, operation, and maintenance. There
The Indiana Limestone Institute wishes to thank the Natural Stone Council for its generous grant, which was used to print this Handbook and to make it available for downloading from our website. TM INDIANA
U.S. DEPARTMENT OF HOUSING AND URBAN DEVELOPMENT R e s i d e n t i a l Rehabilitation Inspection Guide U.S. Department of Housing and Urban Development Office of Policy Development and Research Residential
STAR 193 RLS Bonded Cement Based Material Overlays for the Repair, the Lining or the Strengthening of Slabs or Pavements This publication has been published by Springer in 2011, ISBN 978 94 007 1238 6.
Chicago Southland EPA Brownfields Weatherization Job Training Program STUDENT WORKBOOK This program was funded by the United States Environmental Protection Agency (USEPA) through the American Recovery
1. Report No. FHWA NHI 05-036 4. Title and Subtitle Guidelines for the Installation, Inspection, Maintenance and Repair of Structural Supports for Highway Signs, Luminaires, and Traffic Signals Technical
Pa mphl e t73 At mo s p h e r i cmo n i t o r i n g Eq u i p me n tf o rch l o r i n e Ed i t i o n7 J une2003 Table of Contents 1. INTRODUCTION... 1 1.1 PURPOSE... 1 1.2 RESPONSIBLE CARE... 1 1.3 BACKGROUND...
Pa mphl e t5 Bu l ks t o r a g eo fli q u i d Ch l o r i n e Ed i t i o n8 J une2011 Table of Contents 1. INTRODUCTION... 1 1.1 SCOPE... 1 1.2 CHLORINE INSTITUTE STEWARDSHIP PROGRAM... 1 1.3 DEFINITIONS
Minnesota State Capitol Exterior Stone Repair Project Stone Repair Trials Evaluation and Preliminary Preservation Planning May 10, 2013 Fig. 1. Lion scupper at north roof pediment. The lower portion of
BUYER S GUIDE TO SLAB-ON-GROUND FOUNDATIONS R. Michael Gray, P.E. Matthew T. Gray, EIT 281-358-1121 832-527-6351 email@example.com firstname.lastname@example.org TREC 895 TREC 5904 authors and
Delrin ONLY BY DUPONT Module III acetal resin Design information Registered trademarks of E.I. du Pont de Nemours and Company The miracles of science is a trademark of E.I. du Pont de Nemours and Company
Corrosion Control Many aircraft structures are made of metal, and the most insidious form of damage to those structures is corrosion. From the moment the metal is manufactured, it must be protected from
When you need a floating floor to dramatically Increase your Sound Transmission Class and Impact Noise Rating BULLETIN ACS-102-3.1 Why not use the MASON JACK-UP FLOOR SLAB SYSTEM and eliminate the cost
TILT-UP CONSTRUCTION Fast, Simple, Economical Concrete Construction Method HANDBOOK The economy of tilt-up lies in its simplicity of construction. The critical factors in this method of construction are
Hydraulic Fracturing Operations Well Construction and Integrity Guidelines API GUIDANCE DOCUMENT HF1 FIRST EDITION, OCTOBER 2009 Hydraulic Fracturing Operations Well Construction and Integrity Guidelines
PRODUCT DATA SHEET No.11043/45/46 JANUARY 2002 ISOFLEX HIGH PERFORMANCE LIQUID RUBBER WATERPROOFING SYSTEM The Waterproofing System is based on a moisture curing urethane elastomer. It comprises of three
Glulam P r o d u c t G u i d e 2 A few facts about wood. WOOD The Natural Choice Engineered wood products are a good choice for the environment. They are manufactured for years of trouble-free, dependable
NIST Special Publication 500-252 Information Technology: Care and Handling of CDs and DVDs A Guide for Librarians and Archivists Fred R. Byers Council on Library and Information Resources Washington D.C.
9 Short Guide Maintaining Your Home General ISBN Print: 978-1-84917-182-3 Digital: 978-1-84917-183-0 All images unless otherwise noted are Crown Copyright Principal Authors: Roger Curtis, Moses Jenkins
Managing Steam Sterilization Process By Patricia H. Nothum, RN, BSN, CRCST, CHL A research paper submitted to the International Association of Central Service Health Care Material Management as Partial